Antiviral activity of silver nanoparticle/chitosan composites against H1N1 influenza A virus
© Mori et al.; licensee Springer. 2013
Received: 24 October 2012
Accepted: 1 February 2013
Published: 20 February 2013
Silver nanoparticle (Ag NP)/chitosan (Ch) composites with antiviral activity against H1N1 influenza A virus were prepared. The Ag NP/Ch composites were obtained as yellow or brown floc-like powders following reaction at room temperature in aqueous medium. Ag NPs (3.5, 6.5, and 12.9 nm average diameters) were embedded into the chitosan matrix without aggregation or size alternation. The antiviral activity of the Ag NP/Ch composites was evaluated by comparing the TCID50 ratio of viral suspensions treated with the composites to untreated suspensions. For all sizes of Ag NPs tested, antiviral activity against H1N1 influenza A virus increased as the concentration of Ag NPs increased; chitosan alone exhibited no antiviral activity. Size dependence of the Ag NPs on antiviral activity was also observed: antiviral activity was generally stronger with smaller Ag NPs in the composites. These results indicate that Ag NP/Ch composites interacting with viruses exhibit antiviral activity.
KeywordsOrganic/metal nanocomposites Biomass materials Antimicrobial materials Polysaccharides Nanotoxicity
Silver nanoparticles (Ag NPs) are well-known antimicrobial materials effective against many types of bacteria [1–3] and fungi . The antibacterial and antifungal activities of Ag NPs are mainly due to the inhibition of respiratory enzymes by released Ag+ ions [1, 5]. Recently, the antimicrobial activities of Ag NPs against viruses such as HIV-1 [6, 7], hepatitis B , herpes simplex , respiratory syncytial , monkeypox , Tacaribe , and H1N1 influenza A virus [13, 14] have also been investigated. Unlike its antibacterial and antifungal activities, the major antiviral mechanism of Ag NPs is likely the physical inhibition of binding between the virus and host cell. A dependence of the size of Ag NPs on antiviral activity was observed for the viruses mentioned above; for example, Ag NPs smaller than 10 nm specifically inhibited infection by HIV-1 . This property of Ag NPs holds promise that antimicrobial materials based on Ag NPs will be effective against many types of bacteria, fungi, and viruses.
On the other hand, there are some concerns about the biological and environmental risks of Ag NPs. It is known that Ag NPs have adverse effects, such as cytotoxicity and genotoxicity on aquatic organisms like fish , and can inhibit photosynthesis in algae . One study on mammals showed a significant decline in mouse spermatogonial stem cells following the administration of Ag NPs . Therefore, preventing the diffusion and intake of Ag NPs into the environment and the biosphere are important considerations in the design of antimicrobial materials containing Ag NPs [18–22]. One approach would be the fixation of Ag NPs into matrices; for example, Fayaz et al. have prepared Ag NP-coated polyurethane and have demonstrated its antiviral activity against HIV-1 and herpes simplex virus . Nevertheless, the efficacy and mechanism of action of such Ag NP-fixed antiviral materials against various viral strains are not well investigated.
In this paper, the antiviral activity of Ag NP/polymer composites against H1N1 influenza A virus was investigated. Chitosan (Ch), which is the main constituent of the exoskeleton of crustaceans and exhibits strong antibacterial activity , was used as the matrix polymer. Controlling the size of Ag NPs is as important to antiviral activity as the composition of the Ag NPs. We previously demonstrated an environmentally friendly process for producing Ag NPs with a narrow size distribution . This process uses only three materials: a silver-containing glass powder as an Ag+ supplier, glucose as a reducing agent for Ag+, and water as a solvent. The stabilizing agent for Ag NPs is caramel, which is generated from glucose during heating to reduce Ag+. In this work, Ag NPs synthesized by this process were used to make the Ag NP/Ch composites, since the size of the Ag NPs could be easily controlled without the use or production of hazardous materials. Ag NP/Ch composites were synthesized in aqueous media at room temperature by mixing a chitosan solution and an Ag NP suspension. The surface and internal structure of the synthesized Ag NP/Ch composites were observed by scanning and transmission electron microscopies, respectively. The effect of introducing a small amount of Ag NPs into the chitosan matrices and the effect of the size of the Ag NPs were evaluated with respect to the antiviral activity of the composites.
Characteristics of Ag NPs
Average diameter ± SD (nm)
Concentration of Ag NP in suspension (μg/mL)
3.5 ± 1.8
6.5 ± 1.8
12.9 ± 2.5
Synthesis of Ag NP/Ch composites
Chitosan solution (100 μL, 10 mg/mL) was mixed with Ag NP solution (0.25 to 4.5 mL) and 40 μL 5 M NaOH at room temperature, followed by vigorous stirring to precipitate the Ag NP/Ch composite. The obtained Ag NP/Ch composite was centrifuged at 6,000 rpm for 10 min. The supernatant was analyzed using a UV-visible spectrometer (JASCO V-630, Tokyo, Japan) to estimate the amount of unreacted Ag NPs. Centrifuged composites were washed with 1 mL PBS, followed by centrifugation at 6,000 rpm for 10 min. The washing process was repeated twice. The washed Ag NP/Ch composite was suspended in 250 μL PBS and used in antiviral assays the same day. Synthesis of the Ag NP/Ch composites was carried out in a laminar flow cabinet to prevent biological contamination.
Scanning electron microscopy (SEM) specimens of the composites were prepared by casting 5 μL of a water dispersion of the Ag NP/Ch composite, followed by drying at room temperature. Osmium plasma coating was conducted to enhance the conductivity of the specimens. Dried samples were coated using a plasma multi-coater PMC-5000 (Meiwafosis Co., Ltd., Tokyo, Japan). SEM observation was performed using a JSM-6340F (JEOL, Tokyo, Japan) at 5 kV. Transmission electron microscopy (TEM) specimens of the Ag NPs and Ag NP composites were prepared by casting 5 μL of Ag NP solution or a water dispersion of the composite onto a carbon-coated copper microgrid. Excess solution was removed using filter paper, and the specimens were dried at room temperature. Further staining was not carried out for any specimen. TEM observation was performed using a JEM-1010 (JEOL) at 80 kV.
Assaying the antiviral activity of the Ag NP/Ch composites
Human influenza A virus (A/PR/8/34 (H1N1)), obtained from Life Technologies Co., was used and assayed using the fifty-percent tissue culture infectious dose (TCID50) method. Viral suspension in PBS (250 μL, titer ca. 1,000 TCID50/mL) was added to 250 μL Ag NP/Ch composite suspension. The mixture was stirred vigorously for 5 s and then left at room temperature for 1 h to allow the virus and composite particles to interact. Then, the mixture was centrifuged at 6,000 rpm for 10 min to remove the composite particles. The supernatant (50 μL) was subjected to two-fold serial dilution with PBS 11 times in a 96-well cell culture plate sown with Madin-Darby canine kidney (MDCK) cells. Eight duplicate dilution series were prepared and assayed for each Ag NP/Ch sample. Samples were incubated at 37°C and 5% CO2 for 1 h to allow viral infection of the MDCK cells. MDCK cells were maintained by adding 50 μL DMEM (with the addition of 0.4% of BSA and 5 ppm of trypsin) to each well immediately following infection and again 5 days post-infection. Seven days post-infection, the living cells were fixed with methanol and stained with 5% Giemsa stain solution. The TCID50 of the sample solution was calculated from the number of infected wells using the Reed-Muench method [26, 27]. The antiviral activity of the Ag NP/Ch composite was estimated as the TCID50 ratio of the Ag NP/Ch-treated supernatant to the control (untreated) viral suspension.
Results and discussion
Previous studies showed that Ag NPs have antiviral activity against influenza A virus [13, 14]. Although the mechanism of action has not been well investigated, it is likely that the antiviral activity of Ag NPs against several other types of viruses is due to direct binding of the Ag NPs to viral envelope glycoproteins, thereby inhibiting viral penetration into the host cell [6, 8, 13, 30]. The effect of the size of Ag NPs on antiviral activity was usually observed, suggesting spatial restriction of binding between virions and Ag NPs [6, 8]. For the Ag NP/Ch composites, further spatial restriction due to the chitosan matrix would be expected to prevent or weaken the interaction between virions and Ag NPs. On the other hand, physical binding of virions to the composites could directly inhibit viral contact with host cells since the virus-treated composites were removed from the assay solution prior to infection of the host cells. When embedded Ag NPs could interact with the virions, the interaction between the virions and the composites should increase with increased concentration of Ag NPs in the composites; this is supported by the experimental results on the relationship between the antiviral activity and the concentration of Ag NPs. The effect of the size of Ag NPs in the composites on antiviral activity suggests that influenza A virus interacted selectively with smaller Ag NPs, as previously reported for other types of viruses [6, 8]. However, the size dependence of free Ag NPs on antiviral activity against influenza A virus has not been studied. To obtain more effective Ag NP-embedded antiviral materials, detailed studies of the mechanism of antiviral action of both free and embedded Ag NPs are required. The effects of the microscopic structure and the properties of Ag NP-embedded materials on antiviral activity should also be investigated in the future. Nonetheless, this study clearly demonstrates the feasibility of using Ag NPs to impart antiviral activity to chitosan and lower concerns about the risk of diffusion of Ag NPs in the environment.
Ag NP/Ch composites with antiviral activity against influenza A virus were synthesized in aqueous medium. The composites were obtained as yellow or brown flocs; unreacted Ag NPs were not detected in the residual solution. The particle size of the Ag NPs in the composites was similar to that of the Ag NPs used to synthesize the composites. The antiviral activity of the composites was determined from the decreased TCID50 ratio of viral suspensions after treatment with the composites. For all sizes of Ag NPs tested, the antiviral activity of the Ag NP/Ch composites increased as the amount of Ag NPs increased. Stronger antiviral activity was generally observed with composites containing smaller Ag NPs for comparable concentrations of Ag NPs. Neat chitosan did not exhibit antiviral activity, suggesting that Ag NPs are essential for the antiviral activity of the composites. Although the antiviral mechanism of the composites remains to be investigated, the experimental results showing the relationship between antiviral activity and the concentration of Ag NPs suggest that the virions and composites interacted. Consequently, detailed studies of the antiviral mechanism of the Ag NP/Ch composites could lead to the development of practical Ag NP-containing materials that will reduce concerns about the risks of diffusion of Ag NPs into the environment.
YMo is a technical official of the Japan Air Self-Defense Force. MI and YMi are professors of the National Defense Medical College. TO is a research associate of the National Defense Medical College. TM is a professor of the Tokyo Metropolitan University. VQN is a graduate student of the Tokyo Metropolitan University.
- Ag NP:
Scanning electron microscopy
Transmission electron microscopy
Fifty-percent tissue culture infectious dose.
The authors would like to thank Ms. Y. Ichiki at the Laboratory Center of the National Defense Medical College (Tokorozawa, Japan) for helping with the electron microscopy experiments.
- Pal S, Tak YK, Song JM: Does the antibacterial activity of silver nanoparticles depend on the shape of the nanoparticle? A study of the gram-negative bacterium Escherichia coli. Appl Environ Microbiol 2007, 73: 1712–1720. 10.1128/AEM.02218-06View Article
- Sondi I, Salopek-Sondi B: Silver nanoparticles as antimicrobial agent: a case study on E. coli as a model for Gram-negative bacteria. J Colloid Interface Sci 2004, 275: 177–182. 10.1016/j.jcis.2004.02.012View Article
- Morones JR, Elechiguerra JL, Camacho A, Holt K, Kouri JB, Ramirez JT, Yacaman MJ: The bactericidal effect of silver nanoparticles. Nanotechnology 2005, 16: 2346–2353. 10.1088/0957-4484/16/10/059View Article
- Gajbhiye M, Kesharwani J, Ingle A, Gade A, Rai M: Fungus-mediated synthesis of silver nanoparticles and their activity against pathogenic fungi in combination with fluconazole. Nanomedicine 2009, 5: 382–386. 10.1016/j.nano.2009.06.005View Article
- Liau SY, Read DC, Pugh WJ, Furr JR, Russell AD: Interaction of silver nitrate with readily identifiable groups: relationship to the antibacterial action of silver ions. Lett Appl Microbiol 1997, 25: 279–283. 10.1046/j.1472-765X.1997.00219.xView Article
- Elechiguerra J, Burt JL, Morones JR, Camacho-Bragado A, Gao X, Lara HH, Yacaman M: Interaction of silver nanoparticles with HIV-1. J Nanobiotechnology 2005, 3: 6. 10.1186/1477-3155-3-6View Article
- Trefry JC, Wooley DP: Rapid assessment of antiviral activity and cytotoxicity of silver nanoparticles using a novel application of the tetrazolium-based colorimetric assay. J Virol Methods 2012, 183: 19–24. 10.1016/j.jviromet.2012.03.014View Article
- Lu L, Sun RW, Chen R, Hui CK, Ho CM, Luk JM, Lau GK, Che CM: Silver nanoparticles inhibit hepatitis B virus replication. Antivir Ther 2008, 13: 253–262.
- Baram-Pinto D, Shukla S, Perkas N, Gedanken A, Sarid R: Inhibition of herpes simplex virus type 1 infection by silver nanoparticles capped with mercaptoethane sulfonate. Bioconjugate Chem 2009, 20: 1497–1502. 10.1021/bc900215bView Article
- Sun L, Singh AK, Vig K, Pillai SR, Singh SR: Silver nanoparticles inhibit replication of respiratory syncytial virus. J Biomed Nanotechnol 2008, 4: 149–158.
- Rogers JV, Parkinson CV, Choi YW, Speshock JL, Hussain SM: A preliminary assessment of silver nanoparticle inhibition of monkeypox virus plaque formation. Nanoscale Res Lett 2008, 3: 129–133. 10.1007/s11671-008-9128-2View Article
- Speshock JL, Murdock RC, Braydich-Stolle LK, Schrand AM, Hussain SM: Interaction of silver nanoparticles with Tacaribe virus. J Nanobiotechnology 2010, 8: 19. 10.1186/1477-3155-8-19View Article
- Mehrbod P, Motamed N, Tabatabaian M, Soleimani ER, Amini E, Shahidi M, Kheiri MT: In vitro antiviral effect of "nanosilver" on influenza virus. DARU J Pharm Sci 2009, 17: 88–93.
- Xiang DX, Chen Q, Pang L, Zheng CL: Inhibitory effects of silver nanoparticles on H1N1 influenza A virus in vitro. J Virol Methods 2011, 178: 137–142. 10.1016/j.jviromet.2011.09.003View Article
- Wise JP Sr, Goodale BC, Wise SS, Craig GA, Pongan AF, Walter RB, Thompson WD, Ng AK, Aboueissa AM, Mitani H, Spalding MJ, Mason MD: Silver nanospheres are cytotoxic and genotoxic to fish cells. Aquat Toxicol 2010, 97: 34–41. 10.1016/j.aquatox.2009.11.016View Article
- Navarro E, Piccapietra F, Wagner B, Marconi F, Kaegi R, Odzak N, Sigg L, Behra R: Toxicity of silver nanoparticles to Chlamydomonas reinhardtii. Environ Sci Technol 2008, 42: 8959–8964. 10.1021/es801785mView Article
- Braydich-Stolle LK, Lucas B, Schrand A, Murdock RC, Lee T, Schlager JJ, Hussain SM, Hofmann MC: Silver nanoparticles disrupt GDNF/Fyn kinase signaling in spermatogonial stem cells. Toxicol Sci 2010, 116: 577–589. 10.1093/toxsci/kfq148View Article
- Matyjas-Zgondek E, Bacciarelli A, Rybicki E, Szynkowska MI, Kołodziejczyk M: Antibacterial properties of silver-finished textiles. Fibres Text East Eur 2008, 16: 101–107.
- Filipowska B, Rybicki E, Walawska A, Matyjas-Zgondek E: New method for the antibacterial and antifungal modification of silver finished textiles. Fibres Text East Eur 2011, 19: 124–128.
- Murugadoss A, Chattopadhyay A: A ‘green’ chitosan–silver nanoparticle composite as a heterogeneous as well as micro-heterogeneous catalyst. Nanotechnology 2008, 19: 015603. 10.1088/0957-4484/19/01/015603View Article
- Damm C, Münstedt H: Kinetic aspects of the silver ion release from antimicrobial polyamide/silver nanocomposites. Appl Phys A 2008, 91: 479–486. 10.1007/s00339-008-4434-1View Article
- Sanpui P, Murugadoss A, Prasad PV, Ghosh SS, Chattopadhyay A: The antibacterial properties of a novel chitosan-Ag-nanoparticle composite. Int J Food Microbiol 2008, 124: 142–146. 10.1016/j.ijfoodmicro.2008.03.004View Article
- Fayaz AM, Ao Z, Girilal M, Chen L, Xiao X, Kalaichelvan PT, Yao X: Inactivation of microbial infectiousness by silver nanoparticles-coated condom: a new approach to inhibit HIV- and HSV-transmitted infection. Int J Nanomed 2012, 7: 5007–5018.
- Shi C, Zhu Y, Ran X, Wang M, Su Y, Cheng T: Therapeutic potential of chitosan and its derivatives in regenerative medicine. J Surg Res 2006, 133: 185–192. 10.1016/j.jss.2005.12.013View Article
- Mori Y, Tagawa T, Fujita M, Kuno T, Suzuki S, Matsui T, Ishihara M: Simple and environmentally friendly preparation and size control of silver nanoparticles using an inhomogeneous system with silver-containing glass powder. J Nanopart Res 2011, 13: 2799–2806. 10.1007/s11051-010-0168-zView Article
- Reed LJ, Muench H: A simple method of estimating fifty per cent endpoints. Am J Hyg 1938, 27: 493–497.
- LaBarre DD, Lowy RJ: Improvements in methods for calculating virus titer estimates from TCID50 and plaque assays. J Virol Methods 2001, 96: 107–126. 10.1016/S0166-0934(01)00316-0View Article
- An J, Luo Q, Yuan X, Wang D, Li X: Preparation and characterization of silver-chitosan nanocomposite particles with antimicrobial activity. J Appl Polym Sci 2011, 120: 3180–3189. 10.1002/app.33532View Article
- Sosa IO, Noguez C, Barrera RG: Optical properties of metal nanoparticles with arbitrary shapes. J Phys Chem B 2003, 107: 6269–6275. 10.1021/jp0274076View Article
- Lara HH, Garza-Treviño EN, Ixtepan-Turrent L, Singh DK: Silver nanoparticles are broad-spectrum bactericidal and virucidal compounds. J Nanobiotechnology 2011, 9: 30. 10.1186/1477-3155-9-30View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.